Introducing Manganese-Doped Lead Halide Perovskite Quantum ... · PDF file Crystal...
Embed Size (px)
Transcript of Introducing Manganese-Doped Lead Halide Perovskite Quantum ... · PDF file Crystal...
Introducing Manganese-Doped Lead Halide Perovskite Quantum Dots: A Simple Synthesis Illustrating Optoelectronic Properties of Semiconductors Hanjun Yang, Winnie Fan, Katie Hills-Kimball, Ou Chen,* and Li-Qiong Wang*
Department of Chemistry, Brown University, Providence, Rhode Island 02912, United States
*S Supporting Information
ABSTRACT: Quantum dots (QDs) are considered useful for demonstrating quantum phenomena in undergraduate laboratories due to their monodisperse size and excellent optical properties. Although doping has an increasingly important role in QD fabrication in the semiconductor field, it has rarely been discussed in the context of the undergraduate laboratory. In this work, a simple synthesis and characterization method for Mn-doped CsPbCl3 QDs for an upper-level undergraduate inorganic chemistry laboratory is reported. The Mn-doped CsPbCl3 system benefits from a simplified synthesis and straightforward characterization. This experiment introduces QD research to students and offers opportunities for instructors to discuss many important concepts in inorganic chemistry, such as energy band theory, particle-in-a-box model, electron paramagnetic resonance, ligand field theory, and nanochemistry.
KEYWORDS: Upper-Division Undergraduate, Inorganic Chemistry, Laboratory Instruction, Hands-On Learning/Manipulatives, Crystal Field/Ligand Field Theory, EPR/ESR Spectroscopy, Nanotechnology
■ INTRODUCTION Quantum dots (QD) have been termed as next-generation materials due to their highly tunable electrical, mechanical, electronic, and optical properties, allowing a wide range of applications for displays, photovoltaics, and bioimaging.1−3
Specifically, modern synthetic methods produce monodisperse QDs with well-defined shape, size control, and complex structures, thereby allowing the QDs to emit light at desired frequencies.4−6 Among the various synthetic techniques used to control QD performance, doping, or the intentional introduction of impurity ions within QD lattice, is considered one of the most useful methods due to its wide range of available doping atoms and orthogonality to intrinsic proper- ties.7
Although doping has attracted increasing interest in the nanochemistry field, the concept is yet to be incorporated into undergraduate laboratories due to the complexity in synthesiz- ing doped QDs.8,9 Several chemistry undergraduate laboratory experiments pertaining to QDs have been developed, pioneered by Nordell and Winker.10,11 Currently, the range of QDs in teaching laboratories includes PbS QDs, carbon QDs, and core−shell QDs, etc.12−16 Most of the goals of these laboratory experiments are to demonstrate nanoscale materials to students and discuss size-dependent properties of QDs. Although these laboratory works do vividly present the novelty of QDs and enhance student understanding toward important chemistry ideas, the complex synthesis and characterization methods involved in these works hinder the introduction of the doping concept to the undergraduate audience. The recent development of lead halide perovskite (LHP)
QDs serves as a new platform to present doping to undergraduate laboratory.17−19 LHP requires no complex structure to exhibit the unique properties of the dopant,
which makes characterization easy to accomplish under limited access to instruments.20−22 Additionally, the synthesis of LHP is less time-consuming, allowing students to complete doping QDs within limited laboratory course time without sacrificing the LHP structural integrity. Recently, Shekhirev et al. provided an excellent example of synthesizing CsPbX3 nanocubes in ambient conditions using a teaching lab setup.23 Inspired by the advancements made in LHP studies, we have designed a simple route to synthesize Mn-doped CsPbCl3 QDs in ambient conditions that is suitable for the setup of an upper-level undergraduate chemistry laboratory. By using a simplified hot-injection reaction, students are able to synthesize high-quality Mn-doped CsPbCl3 QDs with bright dopant photoluminescence (PL) and a strong electron paramagnetic resonance (EPR) response. This experiment was developed through the collaboration of
a graduate teaching assistant (TA), an undergraduate student, and faculty members. It was initially tested in Spring 2018 with a small number of students and subsequently implemented successfully in a large inorganic chemistry laboratory course in Spring 2019 at Brown University. Pre- and postexperiment surveys were given to students to assess the learning outcomes. Students were asked to rank the extent of their knowledge of QDs, as well as the synthesis process and spectroscopy used in this experiment, before and after the experiment. The learning goals are to ensure that, upon completing the lab activities, students will be able to
(1) Describe QDs and their basic functions and applications,
Received: September 23, 2018 Revised: July 19, 2019
pubs.acs.org/jchemeducCite This: J. Chem. Educ. XXXX, XXX, XXX−XXX
© XXXX American Chemical Society and Division of Chemical Education, Inc. A DOI: 10.1021/acs.jchemed.8b00735
J. Chem. Educ. XXXX, XXX, XXX−XXX
us t 1
pubs.acs.org/jchemeduc http://pubs.acs.org/action/showCitFormats?doi=10.1021/acs.jchemed.8b00735 http://dx.doi.org/10.1021/acs.jchemed.8b00735
(2) Identify the differences between nanoparticles and bulk crystals,
(3) Synthesize doped QDs, (4) Draw an energy transfer diagram based on ultraviolet−
visible (UV−vis) absorption and PL spectra, (5) Interpret PL spectra and explain the color of doped QDs
observed under the UV irradiation, and (6) Interpret EPR spectra and explain the mechanism for the
observed hyperfine splitting pattern.
Student feedback for the experiment was very positive. This experiment not only allowed students to directly observe the impact of doping in QDs but also provided them with a close link to important concepts introduced in inorganic lectures, including nanomaterials, doping, energy bands, photoexcita- tion, molecular orbitals, and ligand field theory.
■ EXPERIMENTAL SECTION Overview
This experiment is developed by a graduate student TA, with the help of an undergraduate and supervision of faculties. We have successfully implemented this experiment in a large inorganic chemistry laboratory course of 56 students in Spring 2019 at Brown University after piloting it thoroughly with four students in Spring 2018. In the Spring 2019 Inorganic Chemistry Laboratory course, students were divided into four smaller lab sections with the maximum number of students being 16 for each lab section. Students were divided in pairs of two to conduct the synthesis of Mn-doped CsPbCl3 QDs with a given doping concentration. A chart in Figure S1 shows the flow of the different experimental components. This experiment spans across 2 weeks of the lab course. During the first week’s course, students finished the synthesis and purification of doped QDs. In the second week’s course, students characterized their products using UV−vis absorption spectroscopy, PL spectroscopy, and EPR measurements. The detailed lab procedure is provided in Supporting Information. Students were required to read the online lab materials and prepare their lab notebook prior to the start of the lab section. Students were supervised by a graduate teaching assistant (TA) during their 4 h lab section and were given a 30 min prelab lecture by a faculty instructor prior to the experiment. In order to increase the student’s critical, analytical, and writing skills, students were required to write their reports in journal article style and their reports were graded following detailed rubrics. The grading criteria include formatting, organization, data presentation and interpretation, citation, and more (see Supporting Information). Preparation of Cs Oleate
The synthesis of Cs oleate should be conducted prior to the start of the lab by the instructors. A 0.8 g portion of Cs2CO3 was mixed with 40 mL of 1-octadecene (ODE) and 2.5 mL of oleic acid (OA). The mixture was heated to 150 °C under nitrogen protection until the solid was fully dissolved. A pale- yellow clear solution was obtained after 30 min. Prior to student use, the Cs oleate solution should be heated to 120 °C to prevent precipitation. Synthesis of Mn-Doped CsPbCl3 Quantum Dots
A 108 mg portion of PbCl2 was mixed with a desirable amount of MnCl2 with 10 mL of ODE, 1 mL of OA, and 1 mL of oleylamine (OAm) in a three-neck round-bottom flask. The mixture was degassed by bubbling nitrogen gas under vigorous
stirring for 15 min at room temperature. The solution was heated to 120 °C for an hour with continuous nitrogen flow, or until the solid was fully dissolved. The solution was then heated to 180 °C, when 0.8 mL of preheated Cs oleate solution was rapidly injected under vigorous stirring. The reaction was immediately quenched by submerging the product-containing flask in a cold-water bath. As-synthesized QDs were separated from reaction solution by centrifuging at 6000 rpm for 5 min. The precipitate, which contained QDs, was redispersed in hexane or other no